This specification establishes the requirements for electrodeposited tin-nickel alloy coatings from aqueous solutions intended for the corrosion protection of fabricated articles of iron, steel, zinc-base alloys, copper, and copper alloys. This specification does not apply to sheets, strips, or wires in the fabricated form. It also may not be applicable to finely threaded articles, but the decision to use the coating on such components may be made by the purchaser. Coating grades shall be designated by a service condition number, which indicates the severity of exposure for which the coating is intended, and a coating thickness notation. Iron and steel specimens shall undergo pre- and post-coating treatments for reducing the risk of hydrogen embrittlement. Coatings shall be sampled, tested, and conform to specified requirements as to appearance (visible defects), composition, thickness (assessed either by microscopical, magnetic, coulometric, beta backscatter, or X-ray spectrometry), adhesion (determined either by burnishing, or heat-quench test), and integrity (including gross defects, mechanical damage, and porosity).
This abstract is a brief summary of the referenced standard. It is informational only and not an official part of the standard; the full text of the standard itself must be referred to for its use and application. ASTM does not give any warranty express or implied or make any representation that the contents of this abstract are accurate, complete or up to date.
1.1 This specification covers the requirements for electrodeposited tin-nickel alloy coatings from aqueous solutions intended for the corrosion protection of fabricated articles of iron, steel, zinc-base alloys, copper, and copper alloys. The composition of the alloy remains constant at 65/35 tin-nickel in spite of wide fluctuations in both composition and operating conditions. The composition corresponds quite closely to an equiatomic ratio, and the process favors the co-deposition of tin and nickel atoms at identical rates.
1.2 This specification does not apply to sheet, strip, or wire in the fabricated form. It also may not be applicable to threaded articles having basic major diameters up to and including 19 mm because of the nonuniformity of thickness that can be expected on fine threads. However, a decision to use the coating on such components may be made by the purchaser.
1.3 The values stated in SI units are to be regarded as standard. No other units of measurement are included in this standard.
1.4 This standard does not purport to address all of the safety concerns, if any, associated with its use. It is the responsibility of the user of this standard to establish appropriate safety and health practices and determine the applicability of regulatory limitations prior to use.
2. Referenced Documents (purchase separately) The documents listed below are referenced within the subject standard but are not provided as part of the standard.
B183 Practice for Preparation of Low-Carbon Steel for Electroplating
B242 Guide for Preparation of High-Carbon Steel for Electroplating
B246 Specification for Tinned Hard-Drawn and Medium-Hard-Drawn Copper Wire for Electrical Purposes
B252 Guide for Preparation of Zinc Alloy Die Castings for Electroplating and Conversion Coatings
B281 Practice for Preparation of Copper and Copper-Base Alloys for Electroplating and Conversion Coatings
B322 Guide for Cleaning Metals Prior to Electroplating
B374 Terminology Relating to Electroplating
B487 Test Method for Measurement of Metal and Oxide Coating Thickness by Microscopical Examination of Cross Section
B499 Test Method for Measurement of Coating Thicknesses by the Magnetic Method: Nonmagnetic Coatings on Magnetic Basis Metals
B504 Test Method for Measurement of Thickness of Metallic Coatings by the Coulometric Method
B507 Practice for Design of Articles to Be Electroplated on Racks
B567 Test Method for Measurement of Coating Thickness by the Beta Backscatter Method
B568 Test Method for Measurement of Coating Thickness by X-Ray Spectrometry
B571 Practice for Qualitative Adhesion Testing of Metallic Coatings
B602 Test Method for Attribute Sampling of Metallic and Inorganic Coatings
B634 Specification for Electrodeposited Coatings of Rhodium for Engineering Use
B697 Guide for Selection of Sampling Plans for Inspection of Electrodeposited Metallic and Inorganic Coatings
B762 Test Method of Variables Sampling of Metallic and Inorganic Coatings
B765 Guide for Selection of Porosity and Gross Defect Tests for Electrodeposits and Related Metallic Coatings
B809 Test Method for Porosity in Metallic Coatings by Humid Sulfur Vapor (Flowers-of-Sulfur)
B849 Specification for Pre-Treatments of Iron or Steel for Reducing Risk of Hydrogen Embrittlement
B850 Guide for Post-Coating Treatments of Steel for Reducing the Risk of Hydrogen Embrittlement
D3951 Practice for Commercial Packaging
alloys; electrodeposited; tin-nickel; coatings; electrodeposited; nickel alloy; coatings; electrodeposited; tin-nickel alloy; tin-nickel alloy; Burnishing test--for coating adhesion; Coating adhesion--electrodeposited coatings; Copper alloy electrodeposited coatings; Electrodeposited Sn coatings--specifications; Iron products (general)--electrodeposited coatings; Porosity--electrodeposited/metallic coatings; Steel--electrodeposited coatings; Sulfur dioxide (SO2); Tin metals/alloys--electrodeposited coatings; Tin-nickel;
ICS Number Code 25.220.40 (Metallic coatings)
ASTM International is a member of CrossRef.
Citing ASTM Standards
[Back to Top]